advertisement

AIAA JOURNAL Vol. 36, No. 4, April 1998 Modeling of Microcrack Damaged Composite Plates Undergoing Nonlinear Bimodular Flutter Oscillations Taehyoun Kim,¤ Satya N. Atluri,† and Robert G. Loewy‡ Georgia Institute of Technology, Atlanta, Georgia 30332-0356 Numerical methods to investigate the utter response and aeroelastic stability of plates made of composite materials, wherein microcracking occurs in the matrix material, are presented. The analytical modeling of the modulus reduction due to microcracks is based on a self-consistent method with a two-phase model and yields reduced moduli of the composites as functions of the crack density distribution. Both a nite difference and a nite element formulation are presented for two-dimensional laminated plates in supersonic ow. From the numerical results, it is shown that the microcracking in composites results in a loss of aeroelastic stability through nonlinear bimodular oscillation as well as by a direct reduction in the bending stiffness. For three-dimensional utter problems, however, reduction in the torsional rigidity and changes in elastic couplings may further decrease the stability. Nomenclature Ai j Bi j Di j Lij M Mi j Mi0j M1 N t U1 u w x z (k) zn a b p ²i j ²Q i j D ²0 · m k q f ,m 1 r ij r Qi j A m unloaded.Just how little load appearsin the matrix material depends, of course,on the relativemoduli of bers and matrices.Nevertheless, the integrity of the matrix material plays an important structural role of transferring tensile loads around imperfections or damage in an individual ber reinforcement and shear transfer from one ply to another. In particular, high transverse shear exibilities may result in intolerable decay of vibration and utter performances.1 Further, composites designed and used so as to have no major loads in the matrix material cannot provide elastic coupling, and there is widespread agreement that elastic coupling can have substantial bene ts.2 – 5 Elastic couplings, in general, require loading the matrix material in composite laminates. As described by Hill,6 microcracks are responsible for variations in the properties (primarily stiffness) of the constituentmatrix materials. Composite laminates may develop these cracks at load levels well below the failure load under cyclicor monotonic loading conditions. There has been ample research in the development of theories for solids with microcracks.6 – 12 Budiansky and O’Connell7 developed the self-consistent model to determine the elastic moduli of isotropic solids with cracks. Laws et al.8 and Dvorak et al.9 applied this model to calculate reduced moduli of a cracked orthotropic uniply. The analysisof a microcrackeduniply has been used to predict the effect of the damage on the performance of a composite structure. In a series of papers, Makins and Adali13 and Adali and Makins14, 15 used the theory developedin Refs. 8 and 9 to predict the behaviorof cracked laminates in classical plate problems of bending deformation, buckling, and vibration. However, an important feature in the deformation of microcracked laminates, i.e., nonlinear bimodular deformation, was not identi ed during the course of those studies. The investigationof the frequencycharacteristicswas also limited to cross-ply laminates and therefore did not include effects on elastic couplings. Whereas microcracking in the matrix may have a minor effect on the overall elastic properties of the composite structures, the effects on the aeroelastic moduli of structures, particularly those tailored to provide elastic coupling, can be substantial. To the authors’ knowledge, there has been no work reported to this date that properlyaddressessuch issues as they affect the vibration and utter of microcracked laminates. The objectivesof this paper are to identifyand to elucidatethe new nonlinear dynamic phenomenon that arises with microcracked laminated composites and thereby to provide a groundwork for investigation of the effects of transverse microcracks in the matrix on the dynamicand aeroelasticbehaviorof laminatedcompositestructures. = laminate extension moduli as de ned by Eq. (14) = laminate coupling moduli as de ned by Eq. (15) = laminate bending moduli as de ned by Eq. (16) = uniply moduli = number of nite elements = uniply compliances = uncracked uniply compliances = Mach number = number of plies = ply thickness or time = air velocity = longitudinal displacement = lateral displacement = longitudinal coordinate = vertical distance from the midplane to the top of the kth ply = neutral surface location = parameter in Newmark’s scheme = crack density or a parameter in Newmark’s scheme = aerodynamic pressure differential across panel = in-plane strain components in the laminate axes = in-plane strain components in the ply axes = total in-plane strain vector at the midplane = total curvature vector = dynamic pressure or a parameter in Newmark’s scheme = volume fractions of ber and matrix materials, respectively = air density = in-plane stress components in the laminate axes = in-plane stress components in the ply axes I. Introduction LTHOUGH aerospace structures are making greater use of advanced lamentary composite materials than ever before, virtually all of the composites in current use are designed to carry the major loads in bers. That is, matrix material is left largely Received June 16, 1995; revision received Oct. 25, 1997; accepted for c 1998 by the American Institute of publication Nov. 10, 1997. Copyright ° Aeronautics and Astronautics, Inc. All rights reserved. ¤ Research Scientist, Computational Mechanics Center; currently Senior Specialist Engineer, Aeroelastic Analysis, Boeing Commercial Airplane Group, P.O. Box 3707, MS 67-HM, Seattle, WA 98124-2207. Member AIAA. † Institute Professor and Regents’ Professor of Engineering, Computational Mechanics Center. Fellow AIAA. ‡ Professor and Chair, School of Aerospace Engineering. Honorary Fellow AIAA. II. Modeling of Microcracks in a Uniply In a composite laminate, each layer may contain a system of aligned slit cracks that grow in the direction of bers and through 598 599 KIM, ATLURI, AND LOEWY the thickness of the ply, perpendicularto the ply’s plane. The extent of damage is characterized by the formation of new cracks, not by the growth of existing cracks. The formation of microcracks in a ply reduces the stiffness of the ply and, therefore, changes the overall behavior of the laminate. One way to characterize the crack density of a unidirectionalply is by the parameter b D t / s, where t is the ply thickness and s the length between cracks in that ply, assuming that the crack distributionis uniform (Fig. 1). Laws et al.8 and Dvorak et al.9 proposed an analytical modeling of the microcrack in a uniply, and it will be the basis of our modeling of microcracked composite laminates. Depending on the ber diameter relative to an effective medium, one can have either a three-phase or a two-phase model. It is generally known that the predictions of the two models are indistinguishable for most ber-reinforced composites where the ber diameter is much smaller than the crack length.8 According to the two-phase model, the overall stiffness and compliance matrices are given by ¾ D L², ² D M¾ (1) where L D L0 ¡ b N L0 K L (2) M D M0 C b N K bN D 1 4 K D 44 22 D (4) p b 2 Á M11 M 22 ¡ M12 a M 11 where a 1 1 2 1 Ca 1 2 ! and a 2 66 D (5) 2 2 2 Á M11 M22 ¡ M12 M11 M33 ¡ M13 a M 11 K 1 2 1 C a 1 2 ! 2 M55 M66 (6) (7) are the roots of the quadratic equation 2 M 11 M22 ¡ M12 a C M 11 M33 ¡ 2 44 Á £ D0 (8) M11 III. A. 1 2 ! 2 M 55 M 66 (10) (11) Calculation of Reduced Laminate Stiffness For a cracked uniply, the full constitutive equation is 2 3 2 32 3 r 11 ²11 L 11 L 12 L 13 0 0 0 6r 7 6 7 6 L L 0 0 0 7 6²22 7 6 22 7 6 7 22 23 6 7 6 76 7 6r 33 7 6 7 6²33 7 L 33 0 0 0 6 7D6 7 6 7 (12) 6r 23 7 6 6 7 L 44 0 0 7 6 7 6 7 6c 23 7 6 7 6 76 7 L 55 (Symm) 0 5 4c 13 5 4r 13 5 4 r 12 c 12 L 66 In the general analysis of laminated composites, including vibration and utter, it is often adequate to rely on the two-dimensional stress–strain relations based on the classical laminate plate theory (CLPT).17 According to the CLPT, the force resultant-strain relations for a full composite consisting of N plies are N M A(z n ) B(z n ) D where Bi j (z n ) D a) No load Di j (z n ) D and N Z X kD1 N Z X B(z n ) D(z n ) z (k) z (k) k D1 k D1 z (k C 1) N Z X · D [·11 z (k) ²022 ·22 ²0 · (13) L i(k) j dz (14) L (k) i j z dz (15) 2 L (k) i j z dz (16) ° 012 ]T (17) z (k C 1) z (k C 1) ²0 D [²011 ·12 ] T (18) Once microcracks are formed, some of the nonzero entries of the stiffnessmatricesA, B, and D, particularlythose representingelastic couplingterms, will change from their original magnitudes.Further, new coupling terms, such as bending-extension, that did not exist previously may now be present. The neutral plane position z n is de ned by the equation ²11 (z D z n ) D ²110 C z n j c) Tensile (cracks open) Fig. 1 Nonlinear behavior of a microcracked ply. Ca Overall Laminate Stiffness A i j (z n ) D b) Compressive (cracks closed) 1 2 1 The numerical evaluation of M is achieved by performing an iteration method on the preceding equations beginning with M (1) D M0 (Ref. 9). Once the cracked compliance M is evaluated, the cracked stiffness can be obtained by L D M ¡1 . The preceding analysis applies only to cases wherein the cracks remain open. When the microcracksare closed, the quanti cation of the reduced stiffness may be nontrivial.16 In particular, the stiffness matrix does not remain symmetric if slip occurs on crack surfaces. For simplicity, we will assume that the stiffness of a uniply with closed microcracks is equivalent to that of uncracked ply. ¡ [M11 M44 C 2(M11 M13 ¡ M 12 M13 )]a 2 M13 2 2 a M11 M 22 ¡ M12 M11 M 33 ¡ M13 0 M 66 D M 66 C bN (3) The subscript 0 is used to denote the properties of the uncracked composite. The matrix K has only three nonzero components: K Thus, only three compliance coef cients, M22 , M44 , and M66 , are affected by the presence of microcracks, and the remaining coef cients in M are unchanged from their uncracked properties: Á 1 1! 2 M11 M 22 ¡ M 12 a 12 C a 22 0 M22 D M22 C bN (9) M 11 M44 D M 0 C b N 11 D 0 (19) For a two-dimensionalplate with exural bending M11 and in-plane axial load N 11 , B11 M11 ¡ D11 N11 zn D (20) A11 M11 ¡ B11 N 11 600 KIM, ATLURI, AND LOEWY It is probably obvious that, in many cases, A, B, and D are independent of the neutral plane position of the cracked laminate. This is because all of the open cracks are likely to be on either side of the neutralaxis. Exceptionswould be cases where the laminateis loaded by in-plane forces as well as out-of-plane moments, closing only a portion of the cracked zone. In this case, the through-thickness integrations are taken only over the open portion of the cracked plies with the reduced L i j , and the remaining portion is integrated with L 0i j . Evaluation of this new stiffness becomes a nonlinear procedure because the location of the neutral axis itself depends on the true stiffness. In this paper, to simplify our problem, we deal exclusively with simply supported laminates that are free of in-plane load. B. a) b) Crack-Opening Criterion In accordance with our earlier assumption, cracked plies in compression (Fig. 1b) behave as though they are uncracked(b D 0), and those under tension (Fig. 1c) behave according to the crack models. Ultimately, local strain averages at the sites of the cracks will determine the crack opening or closure. In this paper, we adopt the criterion for crack opening or closure as follows: For a cracked ply with index number k and ber angle h (k) , cracks will open if c (k) ²Q22 > 0 c) Fig. 2 Nonlinear bimodular de ection of a microcracked laminate under vertical shear loads. and will close if c (k) ²Q22 < 0 c (k) (k) Here, ²Q22 represents the portion of the total strain ²Q22 in the direction normal to the ber axis that is accommodated by the cracks. The other portion of the total strain is then the average strain of the composite matrix that does not contain any cracks. It can be shown that9 c (k) D b NK ²Q22 22 (k) (k) (k) L (k) Q11 C L (k) Q22 C L (k) Q33 12 ² 22 ² 23 ² (21) where ²Qa (k) b are the total average strains along the material principal axes of the kth ply. Note that, by a coordinate transformation, (k) (k) ²Qa (k)b D la (k) Q c lb Q d ²c d a) No bimodular deformation b) Bimodular deformation (22) where ²c (k)d D ²0c(k)d C z (k) j c d (23) (k) are the total strain components along the laminate axes and la (k) Q c lb Q d are the associated direction cosines. In conjunction with the CLPT, Eq. (21) becomes " # " # 2 (k) L (k) c (k) (k) L 13 (k) (k) (k) 23 Q²22 D b N K 22 L (k) ¡ L Q C L ¡ ²11 ²Q22 12 23 22 (k) L (k) L 33 33 (24) where Mi(k) j are the elements of uniply compliance matrix for the kth ply. IV. Nonlinear Bimodular Deformation In reality, the true distribution of microcracks can be estimated only by static fracture analysis such as given in Ref. 12. The characteristic load to which the laminate is subjected will then determine the degree and locations of the microcracks inside the laminate. In case of a lifting wing or a panel, the structures are frequently loaded by static bending, making their tension sides prone to microcracking. Therefore, without loss of generality, we will assume that all cracks exist on either half side of the cross section. Figure 2a shows a composite plate consisting of a cross-ply laminate with uncracked plies abovethe midsurfacebut with microcrackingin the plies below. Because the stiffness becomes that of either uncracked or cracked laminate, as determined by the local crack-opening/closure status, it is clear that the response of the cracked laminate can become nonlinear. For instance, when the laminate is subjected to shear loads at two different locations as shown in Fig. 2c, its behavior cannot be obtained by simply superimposing the separate responses obtained c) No bimodular deformation Fig. 3 Regions of different deformations on a bimodular momentcurvature curve. under the individualloadingsshown in Figs. 2a and 2b, respectively. Behavior of this nonlinearnature is almost certain to be encountered if the cracked laminate deforms or vibrates about its undeformedposition in which all cracks are just closed. In practice, it is more likely that the cracked laminate will be in a staticallyloaded con guration, which involvescrack openingsor closuresat differentlocationsas an initial condition before any further load is applied. Then the applied load may or may not lead to a nonlinear bimodular deformation, depending on the strain level associated with the load. Examples are shown in Figs. 3a–3c. In this paper, we deal with cracked laminates that vibrate around the at position with small amplitude (Fig. 3b) and hence exhibit the nonlinear bimodular behavior. V. Nonlinear Supersonic Flutter Consider a two-dimensional laminated plate that is simply supported at both ends (Fig. 4). It is assumed that the plate is in nite in its transverse direction and the air ow outside is supersonic. No in-plane axial load is considered, as indicated earlier. We consider all microcracks to be in the plies below the neutral axis of the plate. To derive equations of motion, we assume that a thin-plate theory with Kirchhoff hypothesis can accurately yield the strain energy of the laminate. It is also assumed that the plate has negligible kinetic energy associated with the axial displacement u and 601 KIM, ATLURI, AND LOEWY where a§ ´ k Fig. 4 ¶ 2u ¶ 3w ¡ B(x, t ) D0 2 ¶ x ¶ x3 A(x, t ) (25) ¶ 4w ¶ 3u ¶ 2w D(x, t ) ¡ B(x, t ) 3 C m 2 C D p(x, t ) D 0 4 ¶ x ¶ x ¶ t q D§ p(x, t ) D 2 q 1 U1 2 ¡ M1 ¶ w C ¶ x 1 2 M1 2 M1 ¡2 ¶ w 1 ¢ ¢ ¡ 1 U1 ¶ t 2 3 1 U1 a 2 ¡ 1 M1 ± D b NK 22 22 ± L 90 22 ¡ L 90 22 ± ±2 L 90 23 ± L 90 33 ±2 L 90 ¡ 2390± L 33 90 ²Q22 (27) B(x, t ) D 11 90± 2 11 > 0 < 0 2 ¶ 4 wN Ck ¶ n 4 § Y D by1 Methods of Solution (34) y2 y3 y4 cT ´ bwN wN 0 wN 000c T wN 00 When using Newmark’s scheme,19 the system matrix A§ and the input vector Un are de ned as 2 3 0 1 0 0 0 60 7 0 1 0 0 6 7 A§ D 6 Un D 7, 40 0 0 15 0 § b1§ b2§ 0 0 b§ y C b P1n C b5§ yR1n 1n 3 4 y ) ( (35) where b1§ D ¡ gN § k § ¡ kN c , b (D s ) 2 b D s b2§ D ¡ k N § § b4§ D ( gN § / b D s ) ¡ k N c [1 ¡ (k / b )] § b§ 3 D ¡ b1 , (36) (37) (38) kN § ´ g§ . 2 1 ¡ b§ a§ k § . 2 1 ¡ b§ a§ (39) (40) The boundary conditions at both ends of the laminate are (for all n) y1n (n D 0) D y1n (n D 1) D 0 (41) y3n (n D 0) D y3n (n D 1) D 0 (42) The initial conditions are given as (30) > 0 < 0 ¶ wN ¶ 2 wN C g§ Ck ¶ n ¶ s 2 gN § ´ (29) (31) Here the superscripts § denote uncracked and cracked states, respectively. If an in-plane axial force exists, or if the plate undergoes large de ections during the oscillation, ascertaining crackopening/closure states will be nontrivial. In a nondimensional form, Eqs. (25) and (26) are reduced to the following single equation: b§ a§ ( M1 À 1) ¶ Yn C 1 D A§ Yn C Un ¶ n 90 ± B (D0)I j 11 > 0 B ¡ I j 11 < 0 11 (33) One can employ the central difference (explicit) or Newmark’s (implicit) scheme for the time derivatives wRN and wPN in the governing equation (32). For the (n C 1)th step in time, Eq. (32) can be written in the rst-order form in space as (28) 11 C DCI j D(x, t) D D¡I j 1a m and It can be shown that, for our case, K 22 and L 22 ¡ (L 23 / L 33 ) are al± ways positive. Also, when cracks are open, ¡( B/ A) C z 90 < 0. Thus, cracks will open if j 11 < 0 and will close if j 11 > 0. Accordingly, the stiffness coef cients vary as follows: 11 q l ´ M1 b§ N § [(1/ 2b ) ¡ 1] ¡ k N § c [1 ¡ (k / 2b )]D s 5 D g B ± ¡ C z 90 j A AC I j A¡ I j 0 Finite Difference Method ± 90± A(x, t) D VI. k D0 ma 4 B§a2 D§ h b§ ´ l c ´ , s ´t A. D0 , D§ where In the present study, we do not consider formation of new microcracks during oscillations.Such may actually occur once a dynamic instability is encountered but is beyond the scope of this study. Instead, we concentrate on the initiation of utter. Therefore, the stiffness coef cients will vary with time and space according to the crack-opening criterion discussed in a preceding section. For the case of a cross-ply laminate with cracked plies in the 90-deg direction, Eq. (24) can be approximated as c 90 ’ b NK ²Q22 g§ ´ (26) where A and D are extensional and bending stiffness and B is the bending-extensioncoupling term. From the linear quasisteady theory, the aerodynamic pressure differential across the panel is (for M1 > 1.6) (Ref. 18) 1¡ ´ Two-dimensional orthotropic panel in supersonic ow. crack-opening/closure motion. Thus, one obtains equations of motion for small, geometrically linear deformations in the form D § A§ a 4 , D§h2 § c ¶ wN D0 ¶ s (32) yR10 (n ) D ¡ y10 (n ) D wN 0 (n ) (43) PN 0 (n ) yP10 (n ) D w (44) 1 § § wN 0000 C k N (wN 000 ) wN 00 C k N ( wN 000 )c wPN 0 gN § ( wN 000 ) 0 (45) To solve the nonlinearsystem shown in Eq. (34), the following steps are repeated at each time step (n C 1) ¢D s . 1) Assume y2(n C 1) and y4(n C 1) at n D 0. 2) Integrate from n D 0 to n D 1. 3) At n D 1, check if y1(n C 1) ¼ 0 and if y3(n C 1) ¼ 0. 4) If not, formulate and perform a Newton–Raphson iteration until satis ed. 5) Calculate yP1(n C 1) and yR1(n C 1) . § At each node, the proper gN § and k N , according to the sign of y3(n C 1) (curvature), must be used. 602 B. KIM, ATLURI, AND LOEWY Finite Element Method Suppose that the plate is divided into M elements of equal length lN. It is assumed that the crack-opening/closure state is piecewise constant within each element. That is, cracks in each element are assumed to be either all open or all closed, based on the average curvature of the element. Expressing total strain, kinetic energy, and work in terms of the nondimensional variables and parameters de ned in the preceding sections, the Hamilton principle equation can be written as Z s 2X Z N Z s2X Z N 2 2 M M a § l ¶ uN 1 l ¶ 2 wN d C d dn ds dn ds 2 0 ¶ n 2 2 0 ¶ n s 1 s 1 1 1 ¡d Z ¡ d Z C Z s 2 s 1 s 2 s 1 b Z § 1 s 2 s 1 M X M X 1 2 1 M Z X 1 Z lN k lN 0 lN ¶ uN ¶ 2 wN dn ds ¶ n ¶ n 2 0 0 Nu2 0 0 Nw2 0 N w3 0 Nw4 (48) In the preceding, linear and cubic Hermitian polynomials are used N respectively.19 The vector d contains three nodal disfor uN and w, N w, N wN 0 ) at each end of an element. De ning the strain placements( u, eld vector Bu and Bw as dN u1 Bu ´ 0 0 dn " d2 N w1 d2 Nw2 Bw ´ 0 dn 2 dn 2 dN u2 dn 0 d2 Nw3 dn 2 0 (49) 0 d2 Nw4 dn 2 # leads to the global assembled equation R C CD P C KD D 0 MD (50) (51) where M X g§ m (52) § m (53) (k§ C k § M´ 1 M X C´c K´ M X 1 m´ k§ ´ Z lN 0 Z k 1 lN 0 a) N2T N2 dn BwT Bw C a § BTu Bu ¡ b§ BuT Bw ¡ b§ BTw Bu dn a´ Z lN 0 N2T dN2 dn dn Kn(0)C 1 D Kn 2) Repeat until D(in CC11) ¡ D(i) n C1 ¿ 1 (i) KO n C 1 D KO n C 1 D(i) n C1 (i) R(i) n C 1 D Rn C 1 Dn C 1 Usually, only a few interations are needed at each time step. As mentioned earlier, the crack opening or closure in each element is determined by the sign of the averaged curvature of the element. Although the methods of solution described so far include the effect of bending-extension coupling due to microcracks, this effect can be ignored for practical purposes. Indeed, in all of the numerical examples to follow, the magnitudes of nonzero Bi j are found to be negligible compared with those of Ai j and Di j . Hence, b § ’ 0, gN § ’ g § , k N § ’ k § , and the axial displacement u can be ignored. The nite element formulation for this case simpli es signi cantly. The resulting new formulation is not shown here. VII. A. Results and Discussion Reduced Stiffness of Cross- and Angle-Ply Laminates In the rst part of this section,we presentreduced-stiffnessresults for several symmetric composite laminates under different loading conditions. The undamaged uniply properties are those of VS0054 graphite/epoxy (m f D 0.2 and m m D 0.8) given in Ref. 7. Our purpose is to examine,in qualitativeterms, the overallchangesin the stiffness and compliance of the laminates due to microcracking. We do not intend here an extensive parametric study for a wide variety of crack densities in various plies. Instead, we concentrate on one particular density value, b D 1. (This applies to interior cracked plies. For an outer cracked ply, the effective crack density becomes b D 2.) The rst group of laminates considered are [0/ 90]s and [90/ 0]s cross-ply laminates under the one-dimensional bending moment M11 . The microcrackshave been introduced only in the 90-deg plies below the midsurface (Figs. 5 and 6). Listed next are the A, B, and D matrices for b D 1 as obtained using Eqs. (14–16). Also presented are new neutral axis locations z n expressed in terms of a fraction of the uniply thickness t . As expected, when microcracks exist in the (54) (55) (56) (57) Fig. 5 Crack opening of a [0/90]s laminate. Employing Newmark’s scheme at (n C 1) ¢D s , KO n C 1 Dn C 1 D Rn C 1 (58) where KO n C 1 D Kn C 1 C k 1 Mn C 1 C Cn C 1 b (D s ) 2 b D s (59) Rn ¡ 1 D ¡1 (46) (47) b k 2b Pn CD s ¡ 1 D (0) O (0) D(1) n C 1 D K n C 1 Rn C 1 where d wN dn ds D 0 k C(0) n C 1 D Cn , and solve ¡1 where d ´ [u 1 w1 w10 u 2 w2 w20 ]T and 0 Nw1 Mn(0)C 1 D Mn , (i) D(in CC11) D KO n C 1 R(in C) 1 uN D Nd wN N u1 0 b D s Dn C At each time step, the following iteration is performed. 1) Set dn ds The displacement eld is expressed in terms of shape functions and nodal displacements: N ´ k 1 Rn ¡ 1 D 2b (60) . ¶ wN ¶ wN C c ¶ n ¶ s § C Cn C 1 2 ¶ wN ¶ s g§ 1 1 P Dn C Dn C b (D s ) 2 b D s Rn C 1 D Mn C 1 Fig. 6 Crack opening of a [90/0]s laminate. 603 KIM, ATLURI, AND LOEWY 90-deg layers only, the transverse modulus A 22 changes very little. However, there are signi cant reductionsin other moduli in both the [0/ 90]s and [90/ 0]s laminates. Of particular interest are decreases in the bending stiffness D11 and the torsional stiffness D66 . Furthermore, new bending-extension couplings in the matrix B are now present in the case of cracked laminates. The reduction in the bending stiffness D11 is more prominent for the [90/ 0]s laminate because the cracked 90-deg ply is located farther from the neutral axis than in the [0/ 90]s laminate. Both cross-ply laminates will exhibit the nonlinear bimodular deformation when bent about undeformed, at positions. [0/ 90]s (uncracked): 2 3 40.69 2.21 0 6 7 40.69 0 5 (MN/m) A0 D 4 (Symm) 1.04 2 3 1.661 0.054 0 6 7 0.317 0 5 (N-m) D0 D 4 (Symm) 0.025 B0 D 0, zn D 0 [0/ 90]s (cracked) (0.8% reduction in D11 ): 2 3 40.373 1.664 0 6 7 39.742 0 5 (MN/m) Ac D 4 (Symm) 0.841 2 3 1.647 0.031 0 6 7 0.277 0 5 (N-m) Dc D 4 (Symm) 0.017 2 3 0.064 0.111 0 6 7 0.192 0 5 (kN), z n D 0.012 t Bc D 4 (Symm) 0.040 [90/ 0]s (uncracked): 2 3 40.69 2.21 0 6 7 40.69 0 5 (MN/m) A0 D 4 (Symm) 1.04 2 3 0.317 0.054 0 6 7 1.661 0 5 (kN) D0 D 4 (Symm) 0.025 B0 D 0, Fig. 7 It is seen that both bending and torsion compliances of the cracked laminate will increase, whereas the bending-torsion coupling will decrease. Hence, the degradation of aeroelastic stability could be serious if such a laminate is designed for use in a lifting surface. [§45]s (uncracked): 2 3 22.490 20.411 0 6 7 22.490 0 5 (MN/m) A0 D 4 (Symm) 19.239 2 3 0.547 0.496 0.336 6 7 0.547 0.3365 (N-m), D0 D 4 B0 D 0 (Symm) 0.468 [§45]s (cracked), for M 12 < 0, all cracks close, and for M 12 > 0, all cracks open: 2 3 21.017 19.614 0.012 6 7 21.017 0.012 5 (MN/ m) Ac D 4 (Symm) 19.158 2 3 0.509 0.477 0.342 6 7 0.509 0.3425 (N-m) Dc D 4 (Symm) 0.466 2 3 0.206 0.107 ¡0.022 6 7 0.206 ¡0.0225 (kN) Bc D 4 (Symm) 0.011 Percentage changes in the compliance matrix D¡1 : 2 3 10.7904 ¡9.0040 ¡1.2835 6 7 10.7904 ¡1.28355 (1/ Pa) D¡1 0 D 4 (Symm) 3.9835 2 3 21.0821 ¡19.0028 ¡1.5275 6 7 21.0821 ¡1.52755 (1/ Pa) D¡1 c D 4 (Symm) 4.3926 zn D 0 [90/ 0]s (cracked) (12.7% reduction in D11 ): 2 3 39.742 1.664 0 6 7 40.373 0 5 (MN/m) Ac D 4 (Symm) 0.841 2 3 0.277 0.031 0 6 7 1.647 0 5 (N-m) Dc D 4 (Symm) 0.017 2 3 0.192 0.111 0 6 7 0.064 0 5 (kN), z n D 0.036 t Bc D 4 (Symm) 0.040 The next case is that of the angle-ply laminate [§45]s subjected to the twisting moment M12 . When used for a lifting surface, this laminate will have the bene cial bending-torsion elastic coupling or the so-called washout effect that can be useful in aeroelastic tailoring. It can be shown that, when plies below the midsurface are cracked, all microcracks will close for M 12 < 0 and open for M12 > 0 (Fig. 7). In the following, along with the reduced stiffness, we show estimated percentage changes in the compliance matrices. Crack opening of a [ § 45]s laminate. Increase in the bending compliance: ¡1 Dc11 ¼ 195% ¡1 D011 Increase in the torsion compliance: ¡1 Dc66 ¡1 D066 ¼ 110% Reduction in the bending-torsioncoupling: . ¡1 ¡1 Dc16 Dc11 . ¡1 ¡1 D 016 D011 ¼ 60.9% The observationsand conclusionsdrawn in this section should not be restricted to graphite/epoxy laminates. In other words, depending on the ber and matrix materialsused and their volume fractions,the extent to which the matrix cracks affect various laminate moduli can be quite signi cant. Therefore, an appropriate investigationmust be conducted to adequately de ne the impact of the microcracking. B. Free Vibration Results In the second part of this section, nonlinear bimodular freevibration responses of the microcracked composite laminates that 604 KIM, ATLURI, AND LOEWY Fig. 8 Free vibration responses at » = 0:5 subjected to initial displacement sin(¼»). Fig. 9 Free vibration responses at » = 0:25 subjected to initial displacement sin(2¼»). are in nite in their transverse direction are presented. Because the plates are two dimensional,the longitudinal exural rigidity D11 determines the characteristics of the vibration. Hence, without loss of generality the analysis is limited to the symmetric cross ply [0/ 90]s . Unless indicated otherwise, all results were obtained using eight Hermitian nite elements and Newmark’s integration scheme with k D 0.5 and b D 0.4. Longitudinalmotion due to bending-extension coupling was ignored. Figure 8 shows free vibration responses vs time at the midpoint of both the uncracked and cracked plates. It is assumed that the cracked laminate has a bending stiffness that is 10% smaller than that of the uncracked one. The initial de ection is given in the form of sin(p n ), i.e., the rst vibration mode of the uncracked plate. In this position, all of the cracks are initially closed. Hence, the plate starts to vibrate with the uncracked stiffness D0 . After the rst quarter of its rst cycle, the cracked plate assumes an exact at position in which all cracks are about to open. The plate then moves down with the reduced stiffness Dc , and after a half-cycle it resumes the at position. For the remainder of the cycle, the plate moves with D0 . The subsequentmotion of the cracked plate repeats its rst cycle. This response has a characteristic similar to that of a prismatic bar with bimodular longitudinal stiffness.20 From Fig. 8, it can be seen that the period shifting resulted from the bimodular motion. Also, the maximum peak on the negative side is greater than its counterpart on the positive side. The oscillation shown in Fig. 8 should not be termed nonlinear because each half-period of the motion can be completely predicted by linear analysis. If the initial disturbance displacement is chosen as the second mode sin(2p n ), however, the motion of the cracked plate is quite different, as shown in Fig. 9. Here, there no longer exists smooth shift of motion between the cracked and uncracked plates as crack opening/closure is not uniform along the plate at any instant of motion. The motion is indeed nonlinearbimodular.Figure 10 shows the Fig. 10 Free vibration modes during a half-cycle subjected to initial displacement sin(2¼»). Fig. 11 Free vibration responses at » = 0:25 subjected to initial displacement sin(2¼») using different methods. free-vibration-modeshapes at different instants during a half-cycle subjected to the same initial condition. Because of the nonlinear nature of this oscillation, the mode shapes do not exactly concur at the midpoint. In fact, the location of the node point oscillates. Figures 9 and 10 also indicate that the maximum amplitude level shifts from one part of a cycle to another. Figure 11 represents responses obtained using different methods. To obtain convergence in the nite difference result, it was necessary to put more than 1000 nodes along the plate. For the nite difference result, the time increment of D s D 2.0£10¡2 was used. For the nite element results,20 elements with D s D 0.75 £ 10¡2 for the Newmark method and 12 elements withD s D 0.25 £ 10¡2 for the central difference method were used. Both the nite element and nite difference methods seem to converge well. However, the nite difference method requires much longer computing time because of the large number of nodes required. Figure 12 shows the results of a convergence study using a different number of nite elements for the same cracked plate. The free vibration displacementsare plotted for four such element numbers. Eight elements give results with suf cient accuracy (Fig. 12). C. Flutter Responses and Stability Results In this section, the nonlinear bimodular utter response of the cracked cross-ply laminates considered in the preceding section is explored. All of the responses are subjected to the initial displacement sin(p n ). In Fig. 13, panel utter responses for both cracked and uncracked cross-ply laminates are plotted at k D 303. In both cases, aerodynamic damping is suf ciently dominant to damp out the initial disturbances. However, at k D 328.5, the cracked laminate becomes neutrally unstable(Fig. 14), whereas the uncracked laminate has not yet reached its utter point. Figure 15 shows utter mode shapes of the cracked laminate during a half-cycle of the motion at the critical 605 KIM, ATLURI, AND LOEWY Fig. 12 Convergence of nite element solutions for free vibration responses subjected to initial displacement sin(2¼»). Fig. 13 Flutter responses at » = 0:75 at a pre utter point (¹/M = 0:01; Dc /D0 = 0:9, and ¸ = 303). Fig. 15 Flutter modes at the critical utter point (¹/M = 0:01; Dc /D0 = 0:9, and ¸cr = 328:5). Fig. 16 Flutter responses at » = 0:75 at a post utter point (¹/M = 0:01; Dc /D0 = 0:9, and ¸ = 344:4). Fig. 14 Flutter responses at » = 0:75 at the critical utter point (¹/M = 0:01; Dc /D0 = 0:9, and ¸cr = 328:5). Fig. 17 Flutter responses at » = 0:75 at the critical utter point (¹/M = 0:01; Dc /D0 = 0:8, and ¸cr = 309:2). speed. This utter mode shape resemblesthat of the uncrackedplate. Note that the maximum amplitude occurs at around n D 0.75. But the peak amplitude for wN < 0 is greater than that for wN > 0, as a result of the bimodular oscillation.The effects of nonlinearity,however, do not seem profoundbecause the dominant mode shape is that of the rst vibration mode. It should also be emphasized that, for a given set of parameters, the limit cycle amplitude and frequency are independent of the form of initial conditions. Figure 16 shows a post utter response at k D 344.4, which is the utter boundary for the uncracked laminate. Concerning the cracked laminate behavior in Fig. 14 and the uncracked laminate behavior in Fig. 16, it appears that a 10% reduction in the bending modulus has resulted in about a 5% reduction in the critical dynamic pressure. As might be expected, then, if the stiffness decreases by 20%, the critical dynamic pressure could drop about 10%, as shown in Fig. 17. It appears thus that utter stability of a two-dimensional microcracked laminate as indicated by critical dynamic pressure will be reduced as much as half of the percentage reduction in the bending stiffness. VIII. Conclusion In this study, a nite difference and a nite element model of microcracked composite plates undergoing two-dimensional nonlinear bimodular utter oscillations have been presented using a two-phase, self-consistent crack model and quasisteady supersonic aerodynamic loads. When the microcracked plate deforms about its static con guration in a nonlinear fashion, it is referred to as nonlinear bimodular deformation. As this was a preliminary investigation of such a phenomenon,no attempt has been made to deal with layups 606 KIM, ATLURI, AND LOEWY that are used in actual structures. Numerical simulations in the time domain showed that, for the two-dimensional utter problem, microcracks in composites cause reduced aeroelastic stability through a direct reduction in the bending stiffness and nonlinear bimodular oscillation. However, stiffness results of an angle-ply laminate suggested that microcracking can degrade the aeroelastic stability further by reducing the torsional stiffness and bending-torsioncoupling. Future investigations need to be focused on the in uences of microcracking on elastic couplings as well as various stiffness terms and their potential impact on the aeroelastic performances of realistic composite structures. Acknowledgments The support of this work by the Air Force Of ce of Scienti c Research, with Spencer Wu as the Program Of cial, is gratefully acknowledged. References 1 Birman, V., and Librescu, L., “Supersonic Flutter of Shear Deformable Laminated Composite Flat Panels,” Journal of Sound and Vibration, Vol. 139, No. 2, 1990, pp. 265–275. 2 Ehlers, S. M., and Weisshaar, T. A., “Adaptive Wing Flexural Axis Control,” Proceedings of the Third International Conference on Adaptive Structures, Technomic, Lancaster, PA, 1992, pp. 28–40. 3 Abdelnaser, A. S., and Singh, M. P., “Forced and Random Vibrations of Composite Beams with Bending Torsion Coupling and General Boundary Conditions,” Proceedings of the AIAA/ASME/ASEE/AHS/ASC 34th Structures, Structural Dynamics, and Materials Conference, AIAA, Washington, DC, 1993, pp. 683–692 (AIAA Paper 93-1375). 4 Smith, E. C., “Vibration and Flutter of Stiff-Inplane Elastically Tailored Composite Rotor Blades,” Proceedings of the AIAA/ASME/ASEE/AHS/ASC 34th Structures, Structural Dynamics, and Materials Conference, AIAA, Washington, DC, 1993, pp. 26–37 (AIAA Paper 93-1302). 5 Smith, E. C., and Chopra, I., “Air and Ground Resonance of Helicopters with Elastically Tailored Composite Rotor Blades,” Journal of the American Helicopter Society, Vol. 38, No. 4, 1993, pp. 50–61. 6 Hill, S. C., “A Theory for Predicting and Minimizingthe Effects of Matrix Degradation on the Thermomechanical Properties of General Laminates,” Ph.D. Thesis, Dept. of Mechanical Engineering, Aeronautical Engineering and Mechanics, Rensselaer Polytechnic Inst., Troy, NY, Dec. 1993. 7 Budiansky, B., and O’Connell, R. J., “Elastic Moduliof a Cracked Solid,” International Journal of Solids and Structures, Vol. 12, No. 1, 1976, pp. 81–97. 8 Laws, N., Dvorak, G. J., and Hejazi, M., “Stiffness Changes in Unidirectional Composites Caused by Crack Systems,” Mechanics of Materials, Vol. 2, No. 2, 1983, pp. 123–137. 9 Dvorak, G. J., Laws, N., and Hejazi, M., “Analysis of Progressive Matrix Cracking in CompositeLaminates—I. Thermoelastic Properties of a Ply with Cracks,” Journal of Composite Materials, Vol. 19, No. 3, 1985,pp. 216–234. 10 Fu, Y., and Evans, A. G., “Some Effects of Microcracks on the Mechanical Properties of Brittle Solids—I. Stress, Strain Relations,” Acta Metallurgica, Vol. 33, No. 8, 1985, pp. 1515–1523. 11 Evans, A. G., and Fu, Y., “Some Effects of Microcracks on the Mechanical Properties of Brittle Solids—II. Microcrack Toughening,” Acta Metallurgica, Vol. 33, No. 8, 1985, pp. 1525–1531. 12 Toi, Y., and Atluri, S. N., “Finite Element Analysis of Static and Dynamic Fracture of Brittle Microcracking Solids,” International Journal of Plasticity, Vol. 6, No. 2, 1990, pp. 169–188. 13 Makins, R. K., and Adali, S., “Bending of Cross-Ply Laminated Plates with Matrix Cracks,” Journal of Strain Analysis, Vol. 26, No. 4, 1991, pp. 253–257. 14 Adali, S., and Makins, R. K., “Buckling of Unsymmetrical Cross-Ply Laminates with Matrix Cracks,” International Journal of Mechanical Sciences, Vol. 33, No. 10, 1991, pp. 851–861. 15 Adali, S., and Makins, R. K., “Effect of Transverse Matrix Cracks on the Frequencies of Unsymmetrical Cross-Ply Laminates,” Journal of Franklin Institute, Vol. 329, No. 4, 1992, pp. 655–665. 16 Horii, H., and Nemat-Nasser, S., “Overall Moduli of Solids with Microcracks: Load-Induced Anisotropy,” Journal of the Mechanics and Physics of Solids, Vol. 31, No. 2, 1983, pp. 155–171. 17 Jones, R. M., Mechanics of Composite Materials, McGraw–Hill, New York, 1975, Chap. 4. 18 Dowell, E. H., “Nonlinear Oscillations of a Fluttering Plate,” AIAA Journal, Vol. 4, No. 7, 1966, pp. 1267–1275. 19 Bathe, K., Finite Element Procedures in Engineering Analysis, Prentice–Hall, New York, 1982, Chaps. 5 and 9. 20 Khachatryan, A. A., “Longitudinal Vibrations of Prismatic Bars Made of Different-Modulus Materials,” Mekhanika Tverdogo Tela, Vol. 2, No. 5, 1967, pp. 140–145. R. K. Kapania Associate Editor